#------------------------------------------------------------------------------
#$Date: 2020-07-15 02:30:10 +0300 (Wed, 15 Jul 2020) $
#$Revision: 254288 $
#$URL: file:///home/coder/svn-repositories/cod/cif/8/00/04/8000444.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_8000444
loop_
_publ_author_name
'Zhou, Guojun'
'Liu, Zhiyang'
'Huang, Jinglong'
'Molokeev, Maxim S.'
'Xiao, Zewen'
'Ma, Chonggeng'
'Xia, Zhiguo'
_publ_section_title
;
 Unraveling the Near-Unity Narrow-Band Green Emission in Zero-Dimensional
 Mn²⁺-Based Metal Halides: A Case Study of
 (C₁₀H₁₆N)₂Zn₁₋ₓMn
 x Br₄ Solid Solutions.
;
_journal_name_full               'The journal of physical chemistry letters'
_journal_page_first              5956
_journal_page_last               5962
_journal_paper_doi               10.1021/acs.jpclett.0c01933
_journal_year                    2020
_chemical_formula_moiety
;
2(C10 H16 N), Br4 Mn0.20 Zn0.80
;
_chemical_formula_sum            'C20 H32 Br4 Mn0.2 N2 Zn0.8'
_chemical_formula_weight         683.38
_chemical_name_mineral
;
;
_space_group_IT_number           4
_space_group_name_Hall           'P 2yb'
_space_group_name_H-M_alt        'P 1 21 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 94.958(2)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.5593(4)
_cell_length_b                   9.1402(3)
_cell_length_c                   15.2225(6)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    300
_cell_measurement_theta_max      59.99725
_cell_measurement_theta_min      2.502929
_cell_volume                     1325.07(9)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    8.953
_exptl_crystal_density_diffrn    1.71286(11)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.011
_pd_meas_2theta_range_max        119.9945
_pd_meas_2theta_range_min        5.005858
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        2.56
_pd_proc_ls_prof_wR_expected     2.43
_pd_proc_ls_prof_wR_factor       3.22
_pd_proc_number_of_points        10453.5129
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.33
_refine_ls_R_I_factor            1.17
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            jz0c01933_si_005.cif
_cod_data_source_block           a
_cod_original_cell_volume        1325.08(9)
_cod_original_sg_symbol_Hall
;
P 2yb
;
_cod_original_sg_symbol_H-M      P21
_cod_original_formula_sum
;
C20 H32 Br4 Mn0.20 N2 Zn0.80
;
_cod_database_code               8000444
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z '
'-x, y+1/2, -z '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Mn Mn 0.3618(18) 0.110(2) 0.2317(11) 0.2 3.513579
Zn Zn 0.3618(18) 0.110(2) 0.2317(11) 0.8 3.513579
Br1 Br 0.3724(19) -0.1352(15) 0.2964(10) 1 4.982176
Br2 Br 0.5485(17) 0.143(2) 0.1347(12) 1 8.9616
Br3 Br 0.1319(16) 0.139(2) 0.1492(12) 1 5.969136
Br4 Br 0.3863(18) 0.2976(13) 0.3410(10) 1 5.274316
C1 C 0.19(2) -0.03(2) 0.639(14) 1 5.763849
H1A H 0.10(12) -0.07(14) 0.62(8) 1 8.606295
H1B H 0.17(15) 0.03(14) 0.69(8) 1 8.606295
H1C H 0.25(14) -0.10(12) 0.66(10) 1 8.606295
C2 C 0.37(2) 0.15(2) 0.614(13) 1 6.474461
H2A H 0.44(13) 0.08(16) 0.64(9) 1 9.632733
H2B H 0.34(14) 0.20(16) 0.67(7) 1 9.632733
H2C H 0.40(19) 0.21(16) 0.57(10) 1 9.632733
C3 C 0.28(2) -0.02(3) 0.502(14) 1 5.290108
H3A H 0.35(15) -0.09(14) 0.52(8) 1 7.895683
H3B H 0.33(14) 0.03(13) 0.46(7) 1 7.895683
H3C H 0.21(13) -0.07(14) 0.48(8) 1 7.895683
C4 C 0.140(19) 0.192(18) 0.543(10) 1 4.421583
H4A H 0.12(13) 0.25(11) 0.59(6) 1 5.290108
H4B H 0.19(11) 0.26(11) 0.50(7) 1 5.290108
C5 C 0.003(14) 0.140(16) 0.494(11) 1 3.868885
C6 C 0.002(14) 0.12(3) 0.400(13) 1 5.448021
H6 H 0.08(9) 0.14(14) 0.37(7) 1 6.474461
C7 C -0.13(2) 0.09(2) 0.355(8) 1 7.027158
H7 H -0.13(12) 0.09(19) 0.29(5) 1 8.448381
C8 C -0.24(2) 0.06(2) 0.400(17) 1 8.527338
H8 H -0.32(13) 0.04(15) 0.37(10) 1 10.18543
C9 C -0.239(19) 0.08(3) 0.487(16) 1 8.290467
H9 H -0.32(12) 0.06(18) 0.52(8) 1 9.948561
C10 C -0.11(2) 0.12(3) 0.539(8) 1 5.290108
H10 H -0.10(10) 0.12(17) 0.60(5) 1 6.316546
C11 C 0.37(3) 0.532(17) 0.113(12) 1 5.132194
H11A H 0.38(17) 0.44(12) 0.12(9) 1 7.658813
H11B H 0.42(12) 0.59(16) 0.16(7) 1 7.658813
H11C H 0.43(11) 0.55(13) 0.06(6) 1 7.658813
C12 C 0.16(2) 0.49(2) 0.016(14) 1 4.97428
H12A H 0.21(12) 0.51(14) -0.04(7) 1 7.421942
H12B H 0.07(11) 0.53(12) -0.00(8) 1 7.421942
H12C H 0.16(17) 0.39(11) 0.03(7) 1 7.421942
C13 C 0.23(2) 0.74(2) 0.065(10) 1 4.895324
H13A H 0.28(15) 0.76(14) 0.02(8) 1 7.264029
H13B H 0.26(13) 0.80(15) 0.11(6) 1 7.264029
H13C H 0.13(16) 0.78(13) 0.05(8) 1 7.264029
C14 C 0.15(2) 0.562(16) 0.174(11) 1 3.395144
H14A H 0.20(11) 0.61(14) 0.22(5) 1 4.105755
H14B H 0.15(13) 0.46(10) 0.19(6) 1 4.105755
C15 C -0.005(14) 0.610(19) 0.163(8) 1 3.23723
C16 C -0.109(18) 0.520(17) 0.131(11) 1 4.263669
H16 H -0.09(14) 0.43(12) 0.12(7) 1 5.132194
C17 C -0.248(17) 0.57(2) 0.117(11) 1 5.211151
H17 H -0.32(12) 0.50(14) 0.10(7) 1 6.23759
C18 C -0.286(18) 0.71(2) 0.139(13) 1 5.211151
H18 H -0.38(11) 0.74(11) 0.13(7) 1 6.23759
C19 C -0.18(2) 0.801(19) 0.175(11) 1 4.73741
H19 H -0.21(13) 0.90(10) 0.19(7) 1 5.684892
C20 C -0.039(17) 0.75(2) 0.187(11) 1 3.868885
H20 H 0.03(12) 0.81(10) 0.21(6) 1 4.658453
N1 N 0.246(13) 0.069(14) 0.575(9) 1 3.853093
N2 N 0.225(11) 0.580(16) 0.093(8) 1 3.039838
loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
1.5406 1.0000
1.5443 0.5000
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Br1 Mn Br2 110.6(10) 1_555 1_555
Br1 Mn Br3 108.04(98) 1_555 1_555
Br1 Mn Br4 112.3(10) 1_555 1_555
Br2 Mn Br3 110.39(100) 1_555 1_555
Br2 Mn Br4 107.53(97) 1_555 1_555
Br3 Mn Br4 108.02(97) 1_555 1_555
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mn Br1 2.447(23) .
Mn Br2 2.431(23) .
Mn Br3 2.450(22) .
Mn Br4 2.387(22) .
Zn Br1 2.447(23) .
Zn Br2 2.431(23) .
Zn Br3 2.450(22) .
Zn Br4 2.387(22) .
C1 N1 1.46(23) .
C2 N1 1.48(22) .
C3 N1 1.44(27) .
C4 C5 1.53(21) .
C4 N1 1.56(21) .
C5 C6 1.44(26) .
C5 C10 1.34(22) .
C6 C7 1.41(22) .
C7 C8 1.33(26) .
C8 C9 1.34(35) .
C9 C10 1.45(26) .
C11 N2 1.46(28) .
C12 N2 1.52(24) .
C13 N2 1.53(23) .
C14 C15 1.54(22) .
C14 N2 1.49(20) .
C15 C16 1.35(21) .
C15 C20 1.38(25) .
C16 C17 1.40(22) .
C17 C18 1.38(26) .
C18 C19 1.39(24) .
C19 C20 1.42(23) .
